N A N O R E V I E W
Temperature- and thickness-dependent elastic
moduli of polymer thin films
, Sean Li
The mechanical properties of polymer ultrathin films are usually different from those of their counterparts in bulk. Understanding the effect of thickness on the mechanical properties of these films is crucial for their applications. However, it is a great challenge to measure their elastic modulus experimentally within situheating. In this study, a thermodynamic model for temperature- (T) and thickness (h)-dependent elastic moduli of polymer thin filmsEf(T, h) is developed with verification by the reported experimental data on polystyrene (PS) thin films. For the PS thin films on a passivated substrate,Ef(T,h) decreases with the decreasing film thickness, whenhis less than 60 nm at ambient temperature. However, the onset thickness (h*), at which thicknessEf(T,h) deviates from the bulk value,
can be modulated byT. h* becomes larger at higherTbecause of the depression of the quenching depth, which
determines the thickness of the surface layerδ.
As devices are being developed with a view towards making them smaller, thinner and lighter in dimension, thin polymer films are found to be in more stringent demand in various applications, such as diffusion bar-riers, dielectric coatings, electronic packing, and so on . Therefore, understanding the elastic modulus in confined geometries, such as in thin films, is critical to the stability of the structures of the actual devices. A growing demand exists for the determination of the mechanical properties of thin films and coatings at a rapid pace. Recent researches primarily focusing on the confinement effect of the glass-transition temperature
Tg in thin films [2-7], have presented inconsistent
results. It is believed that such a phenomenon might be attributed to the surface and interfacial effects. However, despite its technological importance, the corresponding elastic modulus of the confined thin polymer films has yet to be fully characterized to the same extent as Tg
effects have been done.
Direct experimental measures of the ultrathin material modulus have proven to be difficult since the presence of stiff substrate tends to interfere with the measure-ments . With regard to the impact of confinement on the elastic modulus of soft materials, there is no
agreement. This occurrence was caused by the various measurement strategies , similar to the initial polymer thin filmTgmeasurements [4,6]. The different trends of
the elastic modulus are due to the different interfacial interactions between probe and the polymer surface. Thus, noncontact mechanics measurement, which does not disturb the free surface, appears to be potentially advantageous for determining the modulus of polymer films. Recently, a wrinkle-based metrology was devel-oped to measure the elastic properties of thin polymer films . In surface wrinkling measurements, to deter-mine the modulus of thin polymer films, a wrinkling instability is utilized to induce compression of a stiff film bonded to a compliant substrate. The film modulus
Ef is determined based on the formula relating the
sub-strate modulus Esub, the film thicknessh, and the
wrink-ling wavelength l: Ef= 3Esub
. At room
temperature, the deduced elastic modulus of the films decreases with decreasing film thickness for ultrathin polymer films (thickness less than 30 nm) . In order to understand better the physical nature of the thickness dependence of the deduced elastic modulus in ultrathin films, a bilayer model was proposed to account for the surface effect on the wrinkling associated with the sur-face of a soft layer .
In the most recent research, the elastic moduli of a series of poly(methacrylate) films with widely varying * Correspondence: firstname.lastname@example.org
School of Materials Science and Engineering, The University of New South Wales, Sydney, NSW 2052, Australia
bulk glass-transition temperature (Tgb) as function of
thickness at ambient temperature were measured by wrinkle-based metrology. A decrease of the modulus was found in all ultrathin polymers films (< 30 nm) with the onset of confinement effects shifting to larger film thicknesses as the quench depth into glass state (Tgb -T) decreases, whereT is the measured temperature . In other words, the quench depth affects the extent of the size dependence. To have a better clarification of the quench-depth effect on the elastic modulus of thin polymer films and the nature of the glass transition of polymers, T was considered as a variant to obtain the temperature-dependent elastic modulus of thin films. However, thein situheating of a polymer-substrate sys-tem covering all the processing and characterization steps is impractical . Therefore, in this study, a model will be developed to investigate the temperature- and thickness-dependent elastic moduli of thin polymer films based on both the bilayer and the size-dependent glass-transition temperature thermodynamic models. The results of this new proposed model are then verified with experimental data that were obtained by wrinkle-based metrology for thin polystyrene (PS) films with dif-ferent molar weights (Mw).
It is well known that the atomic or the molecular struc-ture on a surface is different from the bulk strucstruc-ture in solids. As a result, many materials’properties (e.g., mass density, electrical conductivity, elastic modulus, etc.) on the surface differ from their bulk counterparts. Such a difference is negligible for large-scaled structures. For nanostructures, however, the surface-to-volume ratio is large, and the surface effects can be significant. For thin polymer films of interest in this study, one may assume that a surface layer exists with different elastic moduli. The thickness of the surface layerδmay vary from say one atomic layer for crystalline materials [13-15] to a few nanometers for polymers [16,17]. In the surface layer, lesser density, larger mobility, and softening were found for polymer films [5,17,18]. Therefore, a bilayer model was proposed to describe the elastic modulus of thin polymer filmsEf. In brief, the model consists
of a polymer film with thickness h, containing two dis-tinct moduli. The surface layer of the film has a modu-lus Esur and a finite depth of δ underneath the
atmosphere/solid interface. This depth was considered to be independent of the film thickness. The remainder of the film (h-δ) exhibits a bulk-like modulus (Ebulk).
The bilayer model can be written as 
1− δ h
Esur was considered a few orders of magnitude smaller
than the corresponding Ebulk [11,12]. On the other
hand, it is known that temperature influences the elastic properties of solids [13,19]. In general, the elastic mod-uli of solids would decrease at high temperature due to the weakening of the interactions between atoms or molecules induced by the thermo-expansion of solids . However, Equation 1 ignores the temperature effect, although the mechanical properties of amorphous polymers are slightly influenced by temperature in the glass region. The mechanical properties would change significantly as the temperature approaches theTg.
In addition, the bilayer model considered thatδis inde-pendent of h. However, computer simulations have found that a thinner polymer film has a thicker surface soft layer at a given temperature, and the soft layer would extend to almost the whole film at Tg .
Recent research has shown that the following
relation-ship exists for bulk polymers: δ= 1
Thus,δis related to the quench depth (Tgb -T). In the
nanometer-scale range, the relationship is considered to be still valid since polymer films and corresponding bulk polymer have similar thermodynamic behaviors [18,20]. In addition, simulations have noted that nearTg
the thickness of the free surface layer can nearly extend throughout the thin film . Therefore,
The glass-transition temperature of thin polymer films
Tg(h) is also dependent on the thickness [2-7].
There-fore, after considering temperature effects for T<Tg(h),
the bilayer model can be modified as
It is noted that the temperature effect on the film thickness is ignored in Equation 3 as the thermal expan-sion is relatively small compared with the thickness variation here. In this case,Tg(h) can be determined by
whereh0= 2cξ, withξbeing the correlation length for
which is equivalent to the disappearance of the interface.
as= [2ΔCpb/3R]+1, where Ris the ideal gas constant,
and ΔCpb is the heat-capacity difference between the
bulk glass and the bulk liquid at Tgb.ai=asEs/Eiwith Es and Ei being the bond strength at the surface and
Results and discussion
The theoretical model was applied to the PS thin films to verify the newly developed temperature- and thick-ness-dependent elastic modulus model. First, Ebulk(T)
and Tg(h) should be determined for the PS films. It is
known that the elastic properties decrease almost line-arly in the glass state. They present a very strong tem-perature-dependent behavior nearTg [8,19]. In addition,
generally the glass transition occurs from Tg-50 K for
bulk polymers. Therefore,Ebulk(T) for bulk PS at T<Tg
-50 K is a linear function, which can be deduced from the experimental data obtained from Ebulk(T) =
-0.00189T+ 4.558 . The result is also in agreement with another experimental result where the elastic mod-ulus of bulk PS, Ebulk= 4.0 GPa atT = 294 ± 3 K . Esurwas considered much smaller than the
correspond-ingEbulk; it is about 0.1 GPa for PS .
Figure 1 shows the thickness dependence of the elastic modulus of PS thin films at T = 295 K that was obtained from Equation 3 using expression (4). The parameters needed for the PS thin films are given in the caption of Figure 1. In this figure, our results are com-pared with the corresponding experimental results for
two different molar weights. These results are well in agreement with each other. The modulus for thick films (> 100 nm) was found to be independent of the film thickness, whereas the elastic modulus decreases with the film thickness when the thickness is less than 60 nm. A similar thickness-dependent behavior was also found for several other polymer films, such as poly (methyl methacrylate) (PMMA), poly(ethyl methacrylate) (PEMA), and poly(isobutyl methacrylate) PiBMA [8,11]. The depression of the elastic modulus for thin films is a consequence of the soft surface layer, whose relative importance increases as the surface-to-volume ratio increases.
Using Equation 3, the temperature dependence of elastic modulus of PS thin films with h= 10, 30, and 100 nm and bulk are shown in Figure 2. It is noted that the elastic modulus decreases asT increases for all the films. At low temperatures, there is a nearly linear rela-tionship between the elastic modulus and temperature. However, the elastic modulus decreases steeply at the onset of approximately 210, 300, and 350 K for 10, 30, and 100 nm PS thin films, respectively, while the glass-transition temperatures are 275, 347, and 368 K for 10, 30, and 100 nm, respectively, based on Equation 4. The differences between the onset point andTg are 65, 47,
and 18 K, respectively, for the films of three different thicknesses, which imply that the modulus decreases greatly in the glass-transition temperature region, and this region is more extended as the thickness decreases, consistent with the available experimental data in pub-lished literatures [19,21,22].
Most recently, the deviation of the elastic modulus from its bulk value was studied for thin glassy polymer
0 50 100 150 200
1 2 3 4
Mw = 114 kg/mol Mw = 1800 kg/mol
Figure 1The thickness-dependent elastic modulus of PS thin films atT= 295 K. The symbols circle and square are the experiment results for molar weightMw= 1800 and 114 kg/mol, respectively . The solid curve is plotted with the calculation results obtained from Equation 3, where the parameters that determine theTg(h) in Equation 4 arec= 1/2,h0= 5 nm,ΔCpb= 30.7 J mol-1K-1= 1.919 J g atom-1K-1, andT
gb= 375 K .
0 100 200 300
1 2 3 4 5
(K)10nm 30nm 100nm Bulk
films with different glass-transition temperatures at ambient temperature. These results suggested that the deviations are significantly influenced by the quench depth into the glass (Tgb- T) . To induce the
differ-ent quench depths, the temperatureT is varied in this study. Figure 3 plots the thickness-dependent elastic moduli of PS thin films at different temperatures. For clearly demonstrating the size effect, a relative value of
E(T,h)/E(T,∞) is taken as the ordinate in the figure. From Figure 3, it is found that the size effect is more significant at high temperatures. Recent research has reported that the elastic modulus and glass-transition temperature deviate from the corresponding bulk values at the same thicknesses for poly(n-propyl methacrylate) (PnPMA) thin film on poly(dimethylsiloxane) (PDMS) substrate . In Figure 3,Tg(h)/Tgbfor PS thin films on
a passivated substrate is shown by the dashed curve, which is obtained by Equation 4. We find that the func-tionsTg(h)/TgbandEf(150,h)/E(150,∞) behave in a
simi-lar manner as a function of h. Also, the thicknesses at which the two functions deviate from the corresponding bulk values are almost the same, as in the case of the PnPMA/PDMS system. Considering a criterion that the deviation of the modulus starts when E(T,h)/E(T,∞)≈ 0.96, the critical film thicknessh*, at which the deviation starts for different temperature, is shown in Figure 4. Note thath* increases asTincreases. In other words, at high temperatures, the size effect is more important, and it can be tuned by the application temperature.
Therefore, in actual applications, to avoid decreasing the strength of thin films, one should make sure that the film thickness is larger thanh* for a given temperature. The temperature dependence ofh* is the consequence of the depression of quench depth when the temperature is near the glass-transition region.
The effect of the application temperature on the elas-tic modulus of thin polymer films is seen from the plots of Figure 5, showing the ratioδ/h* as a function of tem-perature. It is noted that this ratio is almost a constant, i.e., approximately 0.004. It is known that the size effect is determined byδ/h, where δis usually considered as independent of h at a given temperature [8,12]. How-ever, Figure 6 shows the surface thickness of PS films of different thicknesses at 295 K as obtained from Equation 2. Thus, δ depends onh and increases ashdecreases. According to Equation 2, it is known thatδis related to
Tg(h), which is dependent on size and can be
deter-mined by Equation 4. In the case of PS films on the pas-sivated substrate, such as on PDMS, where there is no strong interaction between the polymer films and the substrate,Tg(h) decreases with decreasingh. Therefore, δ(h) increases ashdecreases due to the depression ofTg
(h) at a given temperature. On the other hand, the mobility of the polymer film surface layer can be experi-mentally investigated by nanoparticle embedding [17,23] and fluorescence methods . Both methods reported that the surface layer has a thickness of several nan-ometers, which is consistent with the result of Figure 6.
10 20 30 40 50
0.90 0.92 0.94 0.96 0.98 1.00
0.90 0.92 0.94 0.96 0.98 1.00
A theoretical model for the temperature- and thickness-dependent elastic modulus Ef(T,h) was established for
amorphous polymer thin films to investigate the domi-nance of this mechanical property of PS films at nan-ometer scale. We found that at ambient temperature,Ef
(T,h) of PS thin films on the passivated substrate decreases ashdecreases whenhis thinner than 60 nm, whileEf(T,h) is nearly independent on hforh> 60 nm.
Furthermore, a significant thickness effect can be induced by the temperature. The onset of thickness, at whichEf(T,h) deviates from the bulk value, is dependent
on temperature and is larger at high temperature. At a certain temperature, Ef(T,h) exhibits the same
size-dependent trend as Tg(h), which is associated with the
quench depth ofTg(h) -T. Except for the temperature
effect, the thickness of the surface layer also depends on
h, and it increases as h decreases due to the size-dependent glass-transition temperatureTg(h). Therefore, Ef(T,h) of the thin films can be determined using the
developed model, thus providing references for the applications of polymer thin films.
PDMS: poly(dimethylsiloxane); PEMA: poly(ethyl methacrylate); PiBMA: poly (isobutyl methacrylate); PS: polystyrene; PMMA: poly(methyl methacrylate); and PnPMA: poly(n-propyl methacrylate).
This study was supported by the Vice-Chancellor’s Postdoctoral Research Fellowship Program of the University of New South Wales (SIR50/PS19184), the ECR grant of the University of New South Wales (SIR30/PS24201), and the Australian Research Council Discovery Programs DP1096769.
ZA developed the model and drafted the manuscript. SL co-drafted the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Received: 24 September 2010 Accepted: 22 March 2011 Published: 22 March 2011
1. Elshabini-Riad AAR, Barlow FD:Thin Film Technology Handbook.New York: McGraw-Hill; 1997.
2. Keddie JE, Jones RAL, Cory RA:Size-dependent depression of the glass transition temperature in polymer films.Europhys Lett1994,27:59-64. 3. Forrest JA, Dalnoki VK:The glass transition in thin polymer films.Adv
Colloid Interface Sci2001,94:167-195.
4. Jiang Q, Lang XY:Glass transition of low-dimensional polystyrene. Macromol Rapid Commun2004,25:825-828.
5. Ao ZM, Jiang Q:Size effects on miscibility and glass transition temperature of binary polymer blend films.Langmuir2006,22:1241-1246. 6. Alcoutlabi M, McKenna GB:Effects of confinement on material behavior
at the nanometer size scale.J Phys Condens Matter2005,17:R461-R524. 7. Ellison CJ, Torkelson JM:The distribution of glass-transition temperatures
in nanoscopically confined glass formers.Nat Mater2003,2:659-700.
0 100 200 300
0.000 0.002 0.004 0.006 0.008 0.010
Figure 5The ratioδ/h* as a function of temperature.
0 100 200 300
20 40 60
Figure 4The onset thicknessh* of PS films on the passivated substrate at different temperatures.
0 50 100 150 200
2.0 2.5 3.0 3.5 4.0
8. Torres JM, Stafford CM, Vogt BD:Elastic modulus of amorphous polymer thin filmes: Relationship to the glass transition temperature.ACS Nano 2009,3:2677-2685.
9. Forrest JA, Dalnoki-Veress K, Dutcher JR:Brillouin light scattering studies of the mechanical properties of thin freely standing polystyrene films. Phys Phys E1998,58:6109-6114.
10. Stafford CM, Harrison C, Beers KL, Karim AK, Amis EJ, Vanlandingham MR, Kim H-C, Volksen W, Miller RD, Simonyi EE:A buckling-based metrology for measuring the elastic moduli of polymeric thin films.Nat Mater2004, 3:545-550.
11. Stafford CM, Vogt BD, Harrison C, Julhongpiput D, Huang R:Elastic moduli of ultrathin amorphous polymer films.Macromolecules2006,39:5095-5099. 12. Huang R, Stafford CM, Vogt BD:Effect of surface properties on wrinkling
of ultrathin films.J Aerospace Eng2007,20:38-44.
13. Ao ZM, Li S, Jiang Q:The determination of Young’s modulus in noble metal nanowires.Appl Phys Lett2008,93:081905.
14. Sun CQ:Size dependence of nanostructures: impact of bond order deficiency.Prog Solid State Chem2007,35:1-159.
15. Ouyang G, Li XL, Tan X, Yang GW:Size-induced strain and stiffness of nanocrystals.Appl Phys Lett2006,89:031904.
16. Mansfield KF, Theodorou DN:Molecular dynamics simulation of a glassy polymer surface.Macromolecules1991,24:6283-6294.
17. Fakhraai Z, Forrest JA:Measuring the surface dynamics of glassy polymers.Science2008,319:600-604.
18. Bohme TR, de Pablo JJ:Evidence for size-dependent mechanical properties from simulations of nanoscopic polymeric structures.J Chem Phys2002,116:9939-9951.
19. Fukuhara M:Temperature dependency of elastic moduli and internal dilational and shear frictions of polyetherimide.J Appl Polym Sci2003, 90:759-764.
20. Yoshimoto K, Jain T, Nealey PF, de Pablo JJ:Local dynamic mechanical properties in model free-standing polymer thin films.J Chem Phys2005, 122:144712.
21. Ao ZM, Zheng WT, Jiang Q:Lindemann-like size-independent glass-transition criterion for polymers.Polymer2008,49:3578-3581. 22. Tran TA, Saïd S, Grohens Y:Nanoscale characteristic length at the glass
transition in confined syndiotactic poly(methyl methacrylate). Macromolecules2005,38:3867-3871.
23. Ilton M, Qi D, Forrest JA:Using nanoparticle embedding to probe surface rheology and the length scale of surface mobility in glassy polymers. Macromolecules2009,42:6851-6854.
Cite this article as:Ao and Li:Temperature- and thickness-dependent elastic moduli of polymer thin films.Nanoscale Research Letters2011
Submit your manuscript to a
journal and benefi t from:
7 Convenient online submission
7 Rigorous peer review
7 Immediate publication on acceptance
7 Open access: articles freely available online
7 High visibility within the fi eld
7 Retaining the copyright to your article